#------------------------------------------------------------------------------
#$Date: 2016-02-13 14:50:18 +0200 (Sat, 13 Feb 2016) $
#$Revision: 176428 $
#$URL: svn://www.crystallography.net/cod/cif/7/22/08/7220837.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7220837
loop_
_publ_author_name
'Wang, Xiuli'
'Liu, Danna'
'Lin, Hongyan'
'Liu, Guocheng'
'Han, Na'
'Luan, Jian'
'Chang, Zhihan'
_publ_section_title
;
 Application of flexible bis-pyrazine-bis-amide ligands to construct
 various polyoxometalate-based metal-organic complexes
;
_journal_name_full               'RSC Adv.'
_journal_paper_doi               10.1039/C5RA09529H
_journal_year                    2015
_chemical_formula_sum            'C32 H44 Cu2 Mo12 N12 O46 Si'
_chemical_formula_weight         2639.24
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_audit_update_record
;
2015-01-23 deposited with the CCDC.
2015-06-19 downloaded from the CCDC.
;
_cell_angle_alpha                110.9730(10)
_cell_angle_beta                 95.1360(10)
_cell_angle_gamma                117.4280(10)
_cell_formula_units_Z            2
_cell_length_a                   12.3112(7)
_cell_length_b                   12.7440(8)
_cell_length_c                   13.6911(9)
_cell_measurement_temperature    296(2)
_cell_volume                     1694.34(18)
_computing_cell_refinement       'SMART (Bruker, 2001)'
_computing_data_collection       'SMART (Bruker, 2001)'
_computing_data_reduction        'SAINT+ (Bruker, 1999)'
_computing_molecular_graphics    'PLATON (Spek, 2003)'
_computing_publication_material  'SHELXTL (1998)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0157
_diffrn_reflns_av_unetI/netI     0.0271
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            9708
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         1.67
_exptl_absorpt_coefficient_mu    5.760
_exptl_absorpt_correction_T_max  0.4074
_exptl_absorpt_correction_T_min  0.3386
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            GREEN
_exptl_crystal_density_diffrn    5.173
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       BLOCK
_exptl_crystal_F_000             2528
_exptl_crystal_size_max          0.24
_exptl_crystal_size_mid          0.21
_exptl_crystal_size_min          0.19
_refine_diff_density_max         1.670
_refine_diff_density_min         -1.044
_refine_diff_density_rms         0.192
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.051
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     496
_refine_ls_number_reflns         5959
_refine_ls_number_restraints     26
_refine_ls_restrained_S_all      1.050
_refine_ls_R_factor_all          0.0687
_refine_ls_R_factor_gt           0.0641
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1022P)²+33.6855P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1951
_refine_ls_wR_factor_ref         0.1980
_reflns_number_gt                5466
_reflns_number_total             5959
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c5ra09529h2.cif
_cod_data_source_block           liu3
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Triclinic' changed to 'triclinic'
according to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 3271 2015-04-21 07:52:19Z andrius 
;
_cod_original_cell_volume        1694.33(18)
_cod_original_sg_symbol_H-M      'P-1   '
_cod_database_code               7220837
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Mo1 Mo -0.24366(9) -0.06625(10) 0.62724(9) 0.0344(3) Uani 1 1 d .
O1 O -0.8519(7) -0.4386(7) -0.5506(6) 0.0316(16) Uani 1 1 d .
N1 N -0.5644(9) -0.1217(10) 0.0686(7) 0.035(2) Uani 1 1 d .
C1 C -0.5126(12) -0.1956(13) 0.0544(10) 0.045(3) Uani 1 1 d .
Cu1 Cu -0.5000 0.0000 0.0000 0.0376(5) Uani 1 2 d S
O1W O -0.063(3) 0.170(3) 0.949(3) 0.220(12) Uani 1 1 d U
Mo2 Mo 0.05176(10) -0.25406(10) 0.35325(9) 0.0382(3) Uani 1 1 d .
N2 N -0.6750(9) -0.1743(10) -0.1678(8) 0.040(2) Uani 1 1 d .
Cu2 Cu -1.0000 -0.5000 -0.5000 0.0328(4) Uani 1 2 d S
C2 C -0.576(2) -0.392(2) -0.6499(17) 0.098(6) Uani 1 1 d U
H2A H -0.4980 -0.3547 -0.6635 0.118 Uiso 1 1 calc R
O2 O -0.3969(8) -0.0797(8) -0.0396(7) 0.0425(19) Uani 1 1 d .
Mo3 Mo -0.28047(9) -0.01340(10) 0.39294(9) 0.0368(3) Uani 1 1 d .
N3 N -0.6518(16) -0.3225(17) 0.1295(15) 0.083(5) Uani 1 1 d .
O3 O -0.0675(12) -0.1591(14) 0.4113(13) 0.030(3) Uani 0.50 1 d P
C3 C -0.5582(15) -0.2985(16) 0.0819(13) 0.058(4) Uani 1 1 d .
H3A H -0.5239 -0.3519 0.0674 0.070 Uiso 1 1 calc R
Mo4 Mo 0.02161(11) -0.08693(11) 0.71474(9) 0.0407(3) Uani 1 1 d .
N4 N -0.8755(8) -0.3641(8) -0.3565(7) 0.0306(19) Uani 1 1 d .
O4 O -0.0955(13) -0.0283(13) 0.3924(11) 0.027(3) Uani 0.50 1 d P
C4 C -0.6982(16) -0.2446(18) 0.1490(13) 0.066(4) Uani 1 1 d .
H4A H -0.7601 -0.2567 0.1853 0.079 Uiso 1 1 calc R
Mo5 Mo -0.21145(9) -0.32624(10) 0.45662(10) 0.0413(3) Uani 1 1 d .
O5 O -0.1085(12) 0.0293(14) 0.5288(12) 0.026(3) Uani 0.50 1 d P
C5 C -0.6562(13) -0.1448(14) 0.1161(11) 0.049(3) Uani 1 1 d .
H5A H -0.6929 -0.0936 0.1277 0.058 Uiso 1 1 calc R
N5 N -0.3427(13) -0.2156(14) -0.0130(10) 0.061(3) Uani 1 1 d .
H5B H -0.3565 -0.2709 0.0134 0.073 Uiso 1 1 calc R
Mo6 Mo -0.20952(10) -0.24802(11) 0.23393(9) 0.0456(3) Uani 1 1 d .
O6 O -0.0797(12) -0.0859(13) 0.5596(11) 0.026(3) Uani 0.50 1 d P
C6 C -0.8969(11) -0.3312(11) -0.2580(9) 0.036(2) Uani 1 1 d .
H6A H -0.9795 -0.3736 -0.2529 0.043 Uiso 1 1 calc R
N6 N -0.6426(8) -0.2852(9) -0.4967(8) 0.036(2) Uani 1 1 d .
H6B H -0.5738 -0.2258 -0.4422 0.043 Uiso 1 1 calc R
O7 O 0.1828(12) -0.1655(9) 0.4832(8) 0.076(4) Uani 1 1 d .
C7 C -0.7939(11) -0.2335(12) -0.1651(10) 0.040(3) Uani 1 1 d .
H7A H -0.8092 -0.2085 -0.0976 0.048 Uiso 1 1 calc R
O8 O 0.1617(13) -0.1142(9) 0.3142(9) 0.080(4) Uani 1 1 d .
C8 C -0.6549(11) -0.2046(11) -0.2646(9) 0.035(2) Uani 1 1 d .
H8A H -0.5720 -0.1605 -0.2686 0.042 Uiso 1 1 calc R
Si9 Si 0.0000 0.0000 0.5000 0.0263(8) Uani 1 2 d S
O9 O -0.0828(12) -0.2850(18) 0.2392(12) 0.103(6) Uani 1 1 d .
C9 C -0.7547(9) -0.3003(10) -0.3591(8) 0.026(2) Uani 1 1 d .
C10 C -0.7487(9) -0.3451(9) -0.4748(8) 0.027(2) Uani 1 1 d .
O10 O -0.1645(12) 0.0747(10) 0.3212(12) 0.090(5) Uani 1 1 d .
O11 O -0.1188(13) -0.1082(10) 0.2048(13) 0.092(5) Uani 1 1 d .
C11 C -0.632(3) -0.509(4) -0.667(3) 0.151(11) Uani 1 1 d U
H11A H -0.6890 -0.5334 -0.6283 0.181 Uiso 1 1 calc R
O12 O -0.3098(13) -0.1709(10) 0.2884(13) 0.091(5) Uani 1 1 d .
C12 C -0.4148(12) -0.1624(14) -0.0018(10) 0.042(3) Uani 1 1 d .
O13 O -0.3276(13) -0.0776(9) 0.4912(9) 0.086(4) Uani 1 1 d .
C13 C -0.258(3) -0.305(3) -0.150(3) 0.145(10) Uani 1 1 d U
H13A H -0.2641 -0.3650 -0.1202 0.174 Uiso 1 1 calc R
H13B H -0.1838 -0.2811 -0.1765 0.174 Uiso 1 1 calc R
C14 C -0.385(3) -0.378(3) -0.251(3) 0.142(10) Uani 1 1 d U
H14A H -0.4624 -0.4143 -0.2303 0.170 Uiso 1 1 calc R
H14B H -0.3843 -0.3199 -0.2813 0.170 Uiso 1 1 calc R
O15 O -0.2711(12) -0.3389(19) 0.3230(13) 0.111(6) Uani 1 1 d .
C15 C -0.6323(14) -0.3120(16) -0.6082(12) 0.060(4) Uani 1 1 d .
H15A H -0.7176 -0.3565 -0.6584 0.073 Uiso 1 1 calc R
H15B H -0.5807 -0.2278 -0.6094 0.073 Uiso 1 1 calc R
O16 O -0.0919(11) -0.2537(11) 0.6007(10) 0.087(4) Uani 1 1 d .
C16 C -0.2427(16) -0.1880(17) -0.0660(13) 0.064(4) Uani 1 1 d .
H16A H -0.2423 -0.1311 -0.0978 0.076 Uiso 1 1 calc R
H16B H -0.1599 -0.1402 -0.0108 0.076 Uiso 1 1 calc R
O17 O -0.1246(12) -0.0622(11) 0.7214(10) 0.089(5) Uani 1 1 d .
O18 O 0.0775(10) -0.3700(9) 0.2752(8) 0.052(2) Uani 1 1 d .
O19 O -0.3054(9) -0.4809(8) 0.4349(9) 0.053(2) Uani 1 1 d .
O20 O -0.2913(12) -0.2465(12) 0.5258(10) 0.089(5) Uani 1 1 d .
O21 O -0.0719(11) -0.3427(18) 0.4076(12) 0.098(5) Uani 1 1 d .
O22 O -0.3163(9) -0.3631(9) 0.1113(7) 0.052(2) Uani 1 1 d .
O23 O 0.0318(11) -0.1166(12) 0.8230(8) 0.063(3) Uani 1 1 d .
O24 O -0.4081(8) -0.0117(9) 0.3424(9) 0.057(3) Uani 1 1 d .
O25 O -0.3684(8) -0.1057(10) 0.6759(8) 0.057(3) Uani 1 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O25 Mo1 O8 102.6(6) . 2_556
O25 Mo1 O17 103.9(6) . .
O8 Mo1 O17 94.2(5) 2_556 .
O25 Mo1 O13 97.3(6) . .
O8 Mo1 O13 88.2(4) 2_556 .
O17 Mo1 O13 157.5(7) . .
O25 Mo1 O20 98.6(6) . .
O8 Mo1 O20 157.5(7) 2_556 .
O17 Mo1 O20 87.9(4) . .
O13 Mo1 O20 81.6(5) . .
O25 Mo1 O6 157.8(5) . .
O8 Mo1 O6 97.0(6) 2_556 .
O17 Mo1 O6 64.2(6) . .
O13 Mo1 O6 93.4(6) . .
O20 Mo1 O6 63.8(5) . .
O25 Mo1 O5 155.5(5) . .
O8 Mo1 O5 65.4(5) 2_556 .
O17 Mo1 O5 98.5(6) . .
O13 Mo1 O5 62.3(5) . .
O20 Mo1 O5 92.1(6) . .
O6 Mo1 O5 45.1(4) . .
C10 O1 Cu2 113.9(7) . .
C5 N1 C1 118.2(11) . .
C5 N1 Cu1 128.8(9) . .
C1 N1 Cu1 112.8(8) . .
N1 C1 C3 121.2(13) . .
N1 C1 C12 112.6(11) . .
C3 C1 C12 125.9(13) . .
O2 Cu1 O2 179.998(1) 2_455 .
O2 Cu1 N1 82.8(4) 2_455 2_455
O2 Cu1 N1 97.2(4) . 2_455
O2 Cu1 N1 97.2(4) 2_455 .
O2 Cu1 N1 82.8(4) . .
N1 Cu1 N1 179.999(1) 2_455 .
O2 Cu1 N2 89.4(3) 2_455 .
O2 Cu1 N2 90.6(3) . .
N1 Cu1 N2 91.6(4) 2_455 .
N1 Cu1 N2 88.4(4) . .
O2 Cu1 N2 90.6(3) 2_455 2_455
O2 Cu1 N2 89.4(3) . 2_455
N1 Cu1 N2 88.4(4) 2_455 2_455
N1 Cu1 N2 91.6(4) . 2_455
N2 Cu1 N2 179.999(1) . 2_455
O18 Mo2 O21 102.9(6) . .
O18 Mo2 O7 102.1(5) . .
O21 Mo2 O7 93.7(5) . .
O18 Mo2 O9 97.6(6) . .
O21 Mo2 O9 89.4(5) . .
O7 Mo2 O9 158.7(7) . .
O18 Mo2 O8 97.5(5) . .
O21 Mo2 O8 158.8(6) . .
O7 Mo2 O8 87.5(4) . .
O9 Mo2 O8 82.2(5) . .
O18 Mo2 O3 156.4(5) . .
O21 Mo2 O3 65.8(6) . .
O7 Mo2 O3 99.3(6) . .
O9 Mo2 O3 62.9(6) . .
O8 Mo2 O3 93.1(5) . .
O18 Mo2 O5 155.7(5) . 2_556
O21 Mo2 O5 98.5(6) . 2_556
O7 Mo2 O5 64.8(5) . 2_556
O9 Mo2 O5 94.0(6) . 2_556
O8 Mo2 O5 63.0(5) . 2_556
O3 Mo2 O5 46.2(5) . 2_556
C7 N2 C8 118.2(10) . .
C7 N2 Cu1 120.3(8) . .
C8 N2 Cu1 121.2(7) . .
O1 Cu2 O1 180.0(5) 2_344 .
O1 Cu2 N4 96.6(3) 2_344 .
O1 Cu2 N4 83.4(3) . .
O1 Cu2 N4 83.4(3) 2_344 2_344
O1 Cu2 N4 96.6(3) . 2_344
N4 Cu2 N4 180.0(4) . 2_344
C11 C2 C15 121(3) . .
C12 O2 Cu1 112.0(7) . .
O24 Mo3 O13 103.0(6) . .
O24 Mo3 O12 102.1(6) . .
O13 Mo3 O12 93.9(5) . .
O24 Mo3 O10 98.9(6) . .
O13 Mo3 O10 157.3(7) . .
O12 Mo3 O10 87.4(4) . .
O24 Mo3 O7 98.9(5) . 2_556
O13 Mo3 O7 88.0(4) . 2_556
O12 Mo3 O7 157.8(6) . 2_556
O10 Mo3 O7 82.6(5) . 2_556
O24 Mo3 O4 156.8(5) . .
O13 Mo3 O4 97.3(6) . .
O12 Mo3 O4 65.2(6) . .
O10 Mo3 O4 62.7(5) . .
O7 Mo3 O4 92.7(5) 2_556 .
O24 Mo3 O5 158.0(5) . .
O13 Mo3 O5 64.2(5) . .
O12 Mo3 O5 96.8(6) . .
O10 Mo3 O5 93.1(6) . .
O7 Mo3 O5 64.3(5) 2_556 .
O4 Mo3 O5 44.3(5) . .
C4 N3 C3 118.1(14) . .
Si9 O3 Mo2 122.9(7) . .
Si9 O3 Mo6 120.3(6) . .
Mo2 O3 Mo6 96.8(6) . .
Si9 O3 Mo5 119.2(8) . .
Mo2 O3 Mo5 96.3(5) . .
Mo6 O3 Mo5 95.3(5) . .
N3 C3 C1 120.6(14) . .
O23 Mo4 O10 102.3(6) . 2_556
O23 Mo4 O16 102.9(6) . .
O10 Mo4 O16 95.2(5) 2_556 .
O23 Mo4 O17 98.0(6) . .
O10 Mo4 O17 158.2(7) 2_556 .
O16 Mo4 O17 87.6(4) . .
O23 Mo4 O11 97.6(6) . 2_556
O10 Mo4 O11 88.3(5) 2_556 2_556
O16 Mo4 O11 157.9(6) . 2_556
O17 Mo4 O11 81.4(5) . 2_556
O23 Mo4 O6 157.0(5) . .
O10 Mo4 O6 98.9(6) 2_556 .
O16 Mo4 O6 66.1(5) . .
O17 Mo4 O6 62.5(5) . .
O11 Mo4 O6 91.7(6) 2_556 .
O23 Mo4 O4 156.0(5) . 2_556
O10 Mo4 O4 64.0(6) 2_556 2_556
O16 Mo4 O4 98.1(6) . 2_556
O17 Mo4 O4 94.2(6) . 2_556
O11 Mo4 O4 63.9(5) 2_556 2_556
O6 Mo4 O4 45.4(4) . 2_556
C9 N4 C6 118.2(9) . .
C9 N4 Cu2 113.8(7) . .
C6 N4 Cu2 128.0(7) . .
Si9 O4 O5 55.2(6) . .
Si9 O4 Mo3 123.7(8) . .
O5 O4 Mo3 68.6(6) . .
Si9 O4 Mo4 122.4(7) . 2_556
O5 O4 Mo4 130.3(8) . 2_556
Mo3 O4 Mo4 95.5(4) . 2_556
Si9 O4 Mo6 119.4(7) . .
O5 O4 Mo6 132.4(8) . .
Mo3 O4 Mo6 94.5(5) . .
Mo4 O4 Mo6 94.1(5) 2_556 .
N3 C4 C5 121.1(14) . .
O19 Mo5 O20 102.5(6) . .
O19 Mo5 O15 100.6(7) . .
O20 Mo5 O15 94.9(6) . .
O19 Mo5 O16 99.8(5) . .
O20 Mo5 O16 88.3(5) . .
O15 Mo5 O16 158.1(7) . .
O19 Mo5 O21 97.9(6) . .
O20 Mo5 O21 158.4(7) . .
O15 Mo5 O21 88.1(5) . .
O16 Mo5 O21 81.4(5) . .
O19 Mo5 O3 153.8(5) . .
O20 Mo5 O3 99.7(6) . .
O15 Mo5 O3 63.6(6) . .
O16 Mo5 O3 94.6(6) . .
O21 Mo5 O3 62.6(5) . .
O19 Mo5 O6 157.6(5) . .
O20 Mo5 O6 64.3(5) . .
O15 Mo5 O6 98.6(7) . .
O16 Mo5 O6 63.4(5) . .
O21 Mo5 O6 94.2(6) . .
O3 Mo5 O6 47.9(5) . .
Si9 O5 O4 56.5(6) . .
Si9 O5 Mo3 123.4(8) . .
O4 O5 Mo3 67.1(6) . .
Si9 O5 Mo1 122.4(7) . .
O4 O5 Mo1 136.2(8) . .
Mo3 O5 Mo1 94.9(4) . .
Si9 O5 Mo2 120.4(7) . 2_556
O4 O5 Mo2 125.6(8) . 2_556
Mo3 O5 Mo2 94.2(5) . 2_556
Mo1 O5 Mo2 94.0(5) . 2_556
N1 C5 C4 120.7(14) . .
C12 N5 C16 125.5(13) . .
O22 Mo6 O11 101.3(6) . .
O22 Mo6 O9 103.6(6) . .
O11 Mo6 O9 93.9(6) . .
O22 Mo6 O15 100.6(6) . .
O11 Mo6 O15 157.2(7) . .
O9 Mo6 O15 86.9(4) . .
O22 Mo6 O12 97.5(6) . .
O11 Mo6 O12 87.9(5) . .
O9 Mo6 O12 157.9(7) . .
O15 Mo6 O12 83.1(5) . .
O22 Mo6 O3 157.7(5) . .
O11 Mo6 O3 97.7(6) . .
O9 Mo6 O3 63.2(6) . .
O15 Mo6 O3 62.5(6) . .
O12 Mo6 O3 94.8(6) . .
O22 Mo6 O4 154.1(4) . .
O11 Mo6 O4 64.2(5) . .
O9 Mo6 O4 99.0(6) . .
O15 Mo6 O4 93.2(7) . .
O12 Mo6 O4 62.2(5) . .
O3 Mo6 O4 47.4(4) . .
Si9 O6 Mo1 122.7(7) . .
Si9 O6 Mo4 122.7(7) . .
Mo1 O6 Mo4 96.3(5) . .
Si9 O6 Mo5 119.3(7) . .
Mo1 O6 Mo5 94.4(5) . .
Mo4 O6 Mo5 94.4(4) . .
N4 C6 C7 118.8(10) . .
C10 N6 C15 124.6(10) . .
Mo2 O7 Mo3 136.6(7) . 2_556
N2 C7 C6 122.7(11) . .
Mo1 O8 Mo2 137.4(7) 2_556 .
N2 C8 C9 120.9(11) . .
O5 Si9 O5 179.999(4) 2_556 .
O5 Si9 O4 111.7(7) 2_556 .
O5 Si9 O4 68.3(7) . .
O5 Si9 O4 68.3(7) 2_556 2_556
O5 Si9 O4 111.7(7) . 2_556
O4 Si9 O4 180.0(11) . 2_556
O5 Si9 O6 110.4(6) 2_556 .
O5 Si9 O6 69.6(6) . .
O4 Si9 O6 110.7(7) . .
O4 Si9 O6 69.3(7) 2_556 .
O5 Si9 O6 69.6(6) 2_556 2_556
O5 Si9 O6 110.4(6) . 2_556
O4 Si9 O6 69.3(7) . 2_556
O4 Si9 O6 110.7(7) 2_556 2_556
O6 Si9 O6 179.998(3) . 2_556
O5 Si9 O3 109.8(7) 2_556 2_556
O5 Si9 O3 70.2(7) . 2_556
O4 Si9 O3 107.3(7) . 2_556
O4 Si9 O3 72.7(7) 2_556 2_556
O6 Si9 O3 106.8(7) . 2_556
O6 Si9 O3 73.2(7) 2_556 2_556
O5 Si9 O3 70.2(7) 2_556 .
O5 Si9 O3 109.8(7) . .
O4 Si9 O3 72.7(7) . .
O4 Si9 O3 107.3(7) 2_556 .
O6 Si9 O3 73.2(7) . .
O6 Si9 O3 106.8(7) 2_556 .
O3 Si9 O3 179.999(2) 2_556 .
Mo6 O9 Mo2 136.9(9) . .
N4 C9 C8 121.1(10) . .
N4 C9 C10 111.3(8) . .
C8 C9 C10 127.5(10) . .
O1 C10 N6 121.2(10) . .
O1 C10 C9 117.5(9) . .
N6 C10 C9 121.2(9) . .
Mo4 O10 Mo3 137.5(8) 2_556 .
Mo6 O11 Mo4 137.4(8) . 2_556
C2 C11 C14 127(3) . 2_444
Mo3 O12 Mo6 138.0(8) . .
O2 C12 N5 119.0(12) . .
O2 C12 C1 119.6(10) . .
N5 C12 C1 121.4(12) . .
Mo3 O13 Mo1 138.0(8) . .
C16 C13 C14 111(3) . .
C11 C14 C13 99(3) 2_444 .
Mo5 O15 Mo6 138.6(9) . .
C2 C15 N6 116.1(16) . .
Mo4 O16 Mo5 135.9(7) . .
C13 C16 N5 113.4(19) . .
Mo1 O17 Mo4 136.7(8) . .
Mo5 O20 Mo1 137.3(8) . .
Mo2 O21 Mo5 134.9(8) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Mo1 O25 1.664(8) .
Mo1 O8 1.830(10) 2_556
Mo1 O17 1.832(10) .
Mo1 O13 1.970(10) .
Mo1 O20 1.970(10) .
Mo1 O6 2.372(13) .
Mo1 O5 2.404(13) .
O1 C10 1.263(12) .
O1 Cu2 1.928(7) .
N1 C5 1.323(16) .
N1 C1 1.331(16) .
N1 Cu1 1.990(10) .
C1 C3 1.37(2) .
C1 C12 1.466(18) .
Cu1 O2 1.963(8) 2_455
Cu1 O2 1.963(8) .
Cu1 N1 1.990(10) 2_455
Cu1 N2 2.430(9) .
Cu1 N2 2.430(9) 2_455
Mo2 O18 1.670(9) .
Mo2 O21 1.835(11) .
Mo2 O7 1.848(10) .
Mo2 O9 1.958(11) .
Mo2 O8 1.971(10) .
Mo2 O3 2.326(13) .
Mo2 O5 2.438(14) 2_556
N2 C7 1.314(15) .
N2 C8 1.321(15) .
Cu2 O1 1.928(7) 2_344
Cu2 N4 1.946(9) .
Cu2 N4 1.946(9) 2_344
C2 C11 1.23(4) .
C2 C15 1.47(2) .
O2 C12 1.274(15) .
Mo3 O24 1.672(8) .
Mo3 O13 1.819(10) .
Mo3 O12 1.841(10) .
Mo3 O10 1.957(10) .
Mo3 O7 1.965(9) 2_556
Mo3 O4 2.372(13) .
Mo3 O5 2.398(13) .
N3 C4 1.32(2) .
N3 C3 1.34(2) .
O3 Si9 1.667(14) .
O3 Mo6 2.384(15) .
O3 Mo5 2.393(13) .
Mo4 O23 1.663(9) .
Mo4 O10 1.821(11) 2_556
Mo4 O16 1.846(10) .
Mo4 O17 1.969(11) .
Mo4 O11 1.973(11) 2_556
Mo4 O6 2.372(13) .
Mo4 O4 2.385(14) 2_556
N4 C9 1.338(13) .
N4 C6 1.351(15) .
O4 Si9 1.612(13) .
O4 O5 1.80(2) .
O4 Mo4 2.385(14) 2_556
O4 Mo6 2.450(14) .
C4 C5 1.39(2) .
Mo5 O19 1.653(8) .
Mo5 O20 1.814(11) .
Mo5 O15 1.831(11) .
Mo5 O16 1.958(11) .
Mo5 O21 1.971(10) .
Mo5 O6 2.434(14) .
O5 Si9 1.589(13) .
O5 Mo2 2.438(14) 2_556
N5 C12 1.333(16) .
N5 C16 1.453(19) .
Mo6 O22 1.662(8) .
Mo6 O11 1.826(11) .
Mo6 O9 1.828(12) .
Mo6 O15 1.942(10) .
Mo6 O12 1.950(10) .
O6 Si9 1.619(13) .
C6 C7 1.378(16) .
N6 C10 1.301(14) .
N6 C15 1.471(17) .
O7 Mo3 1.965(9) 2_556
O8 Mo1 1.830(10) 2_556
C8 C9 1.370(14) .
Si9 O5 1.589(13) 2_556
Si9 O4 1.612(13) 2_556
Si9 O6 1.619(13) 2_556
Si9 O3 1.667(14) 2_556
C9 C10 1.501(15) .
O10 Mo4 1.821(11) 2_556
O11 Mo4 1.973(11) 2_556
C11 C14 1.59(4) 2_444
C13 C16 1.43(3) .
C13 C14 1.60(4) .
C14 C11 1.59(4) 2_444
